2Casting Methods • Sand Casting High Temperature Alloy, Complex Geometry,Rough Surface Finish• Investment CastingHigh Temperature Alloy,Complex Geometry,Moderately Smooth SurfaceFinish• Die CastingHigh Temperature Alloy,Moderate Geometry,Smooth Surface
3Sand CastingMetals: Most castable metals.Size Range: Limitation depends on foundry capabilities. Ounces to many tons.Tolerances:Non-Ferrous ± 1/32² to 6²Add ± .003² to 3², ± 3/64² from 3² to 6².Across parting line add ± .020² to ± .090² depending on size.(Assumes metal patterns)Surface Finish:Non-Ferrous: RMSFerrous: RMSMinimum Draft Requirements:1° to 5°Cores: 1° to 1 1/2°Normal Minimum Section Thickness:Non-Ferrous: 1/8² - 1/4²Ferrous: 1/4² - 3/8²
5Three Cast Structures of Solidified Metals FIGURE Schematic illustration of three cast structures of metals solidified in a square mold:(a) pure metals;(b) solid-solution alloys; and(c) the structure obtained by heterogeneous nucleation of grains, using nucleating agents.
14Sand Casting Process Pattern (oversized to allow for shrinkage) Ramming sand around Pattern in a FlaskCompacting / jolting sand (green sand, skin dried or, loam moulded)Withdraw Pattern, add CoreReassemble Mould, with Gating, Runner, Riser, and SprueWeight and ready for pouring.
15Process Parameters Pouring Temperature Cooling rate Fluidity (viscosity)Grain StructureLimit of flow before freezingSpiral mould
30Sand Casting - ProsProduce parts with complex geometries, both internally and externally.Possible to net shape with no further manufacturing required.Large parts can be produced.Wide choice of metals.Suitable for mass production.
31Sand Casting - Cons Porosity Poor dimensional control for some processesPoor surface finish for some processesLimitation on mechanical propertiesSafety hazardEnvironmental hazard
33Casting Quality - Defects Misruns - unfilled region existsinsufficient fluidity of meltlow pouring temperatureslow pouringcross-section too thinCold shut - premature freezing at fusion point. Similar reason as misrun
34Casting Quality - Defects Cold shots - Splattering during pouring forming solid globules. Redesign of pouring procedure or gating system is needed.Shrinkage cavity - depression or internal void caused by solidification shrinkage. Solved by proper riser design.
35Casting Quality - Defects Microporosity -Network of small voids caused by localised solidification shrinkage. Caused by the freezing manner of the alloy.Hot tearing - Occurs at location with high stress due to inability to shrink naturally. Resolve by mold collapsing or removing from the mold immediately after freezing.
36Casting Quality - Defects (Sand Casting) Sand blow - cavity caused by mold gas during pouring. Low permeability, poor venting or high moisture content.Pin holes - small gas cavities.Sand wash - erosion of sand mold during pouring.Scabs - mold surface locally flakes off and embedded in the casting during solidification.
37Casting Quality - Defects (Sand Casting) Penetration - penetration of molten metal into the sand. Harder packing of sand is needed.Mold shift - shift of the cope relative to the drag.Core shift - shift of the core, usually vertical.Mold crack - mold strength insufficient, liquid metal form a fin of the final casting.
38Product Design Considerations Geometric simplicity - Avoid unnecessary complexity.Corners - Avoid sharp corners, generous fillet radius.Section thickness - Uniform section thickness to avoid shrinkage cavities and hot spots.Draft - Facilitate removal of parts from mold. (1 deg. For sand and 2/3 deg. for permanent)Use of cores - minimize the use of coreDimensional tolerance and surface finish - proper choice of casting method.Machining allowances - For assembly purposes, typically 1.5 to 6 mm.
39Product Design Considerations Shrinkage, hot spotDraft and core elimination
46Investment CastingFIGURE Schematic illustration of investment casting (lost-wax process). Castings by this method can be made with very fine detail and from a variety of metals. Source: Steel Founders’ Society of America.
50Expendable Mold Casting - Investment Casting Pros:Capability to cast parts with great complexity and intricacy.Close dimensional control ( m tolerance).Good surface finish.Wax can be recovered and reuse.Additional machining normally not required.Cons:Normally cater for smaller parts.Relatively expensive
51Expendable Pattern Casting Figure Schematic illustration of the expendable pattern casting process, also known as lost foam or evaporative casting. Pattern made from Polystrene and vaporized when in contact with molten metal. The pattern can include the sprue and runner. No cope / drag is needed.
53Expendable Mold Casting - Expanded Polystrene Mold Pros:Pattern need not be removed.No cope /drag is needed, all features are built into the pattern.Possibility for automated production.Cons:The pattern is not reusable.
54Operation Sequence of Making a Ceramic Mold FIGURE Sequence of operations in making a ceramic mold.
55Figure 11.17 A typical ceramic mold (Shaw process) for casting steel dies used in hot forging.
56Expendable Mold Casting - Plaster Mold and Ceramic Mold Similar to sand casting in terms of process.Plaster mold is for lower temperature alloys while ceramic mold is for higher temperature alloys.Pros:Good surface finish and dimensional control.Capability to make thin cross sections.Cons:Curing takes too long to render it unsuitable for volume production.
57ٍShell Casting Dump-Box Technique Figure A common method of making shell molds. Called dump-box technique, the limitations are the formation of voids in the shell and peelback (when sections of the shell fall off as the pattern is raised). Source: ASM International.
59Expendable Mold Casting - Shell Mold Pros:Smoother surface finish than sans casting.Surface finish of 2.5 m can be obtained.Good dimensional accuracy 0.25 mm on small to medium size parts.No further machining is needed.Capability for automation lowers the cost for larger quantities.Cons:More expensive metal pattern, especially for small batch.
60Expendable Mold Casting - Vacuum Mold 1. Thin pre-heated plastic sheet sucks onto the vacuum vented pattern surface.2. Special flask with vents and filled with sand is placed over the pattern.3. Another plastic sheet covers the sand and vacuum is drawn.
61Expendable Mold Casting - Vacuum Mold 4. Vacuum on the pattern is released to free the sand mold.5. Cope and drag is assembled to form the complete mold. The plastic sheet is burnt away when in contact with the molten metal.
62Vacuum-Casting Process FIGURE Schematic illustration of the vacuum-casting process. Note that the mold has a bottom gate. (a) Before and (b) after immersion of the mod into the molten metal. Source: After R. Blackburn.
63Expendable Mold Casting - Vacuum Mold Sand held together by vacuum pressure.Pros:Sand can be recovered unlike shell mold.No chemical binder, and therefore no special treatment for the sand.No water mixed with the sand and therefore no moisture related problemsCons:Relative slowNot readily adaptable to mechanization.
66Pressure-Casting Process FIGURE The pressure-casting process uses graphite molds for the production of steel railroad wheels. Source: Griffin Wheel Division of Amsted Industries Incorporated.
67Permanent Mold Casting - Basic Permanent Mold Pros:Good surface finish and close dimensional control.More rapid solidification, finer grain structure, stronger castings.Cons:Generally limited to lower melting point metals.Simpler part geometries as mold is permanent.Mold cost is expensive and thus cater for volume production.
68Permanent Mold Casting - Die Casting Hot-chamber machines :Metal molten in container attached to machine. Typical injection pressures are 7 to 35 MPa. The piston is subjected to the melting temperature of the metal and thus the process is often used for low melting point metals such as zinc, tin, lead or magnesium alloys.Cold-chamber machinesMolten metal is poured into an unheated chamber from an external container. Typical injection pressures are 14 to 140 MPa. Often used for high melting point metal such as aluminum, brass, and magnesium alloys.
69Die Casting in Hot-Chamber Process FIGURE Sequence of steps in die casting of a part in the hot-chamber process. Source: Courtesy of Foundry Management and Technology.
70Die Casting in Cold-Chamber Process FIGURE Sequence of operations in die casting of a part in the cold-chamber process.
73Permanent Mold Casting - Die Casting Mold made of tool steel.Mold opening mechanism to be synchronized with ejector pins.Venting is needed for air and gas typically at the parting surface.Flash formation is common.
74Permanent Mold Casting - Die Casting Pros:High production rates are possible.Economical for large quantities.Close tolerances are possible ( mm).Good surface finish.Thin sections are possible (down to 0.5 mm).Rapid cooling, fine grain, high strength.Cons:melting point of metals.shape restriction.
75Centrifugal Casting Process FIGURE Schematic illustration of the centrifugal casting process. Pipes, cylinder liners, and similarly shaped parts can be cast by this process.
76Semicentrifugal Casting Process FIGURE (a) Schematic illustration of the semicentrifugal casting process. (b) Schematic illustration of casting by centrifuging. The molds are placed at the periphery of the machine, and the molten metal is forced into the molds by centrifugal forces.